preparation and characterization of ...eprints.utm.my/id/eprint/32448/1/...yang berbeza semasa suhu...
Click here to load reader
Post on 24-May-2019
Embed Size (px)
PREPARATION AND CHARACTERIZATION OF POLYACRYLONITRILE
FIBER PRECURSOR USING MULTI-HOLE SPINNERET
DAYANG SALYANI BINTI ABANG MAHMOD
A thesis submitted in fulfilment of the
requirements for the award of the degree of
Master of Engineering (Gas)
Faculty of Petroleum and Renewable Energy Engineering
Universiti Teknologi Malaysia
To my beloved parent,
(Abang Mahmod Bin Abang Kipli and Salha Binti Majid)
(Abang Mahzrie, Abang Mohd Fardaus and Dayang Zafirah)
and relatives for their inspirational words, best encouragement, undoubted feelings,
mind and endless support, inspired and motivated me
throughout the success of this research study.
First and foremost, I would like to express my deep and sincere gratitude to
my dedicated supervisors; Prof. Dr. Ahmad Fauzi Ismail and Associate Prof. Dr.
Azeman Mustafa for their wide knowledge and personal guidance which have been
of great value for me, for their detailed and constructive comments and also for
encouraging me in this endeavor. I also wish to express warm and sincere thanks to
Dr. Mohamed G. Abdallah (Consultant, MGA-Advanced Composites & Engineering) and
Emeritus Prof. Takeshi Matsuura (University of Otawa, Canada) who gave me
important guidance during my research and writing manuscripts. I wish to
acknowledge the encouragement past and present members of our laboratory at
AMTEC whose enthusiastic cooperation and very important work were for me the
best support during this long and sometimes difficult venture, have helped towards
my completion of this master study. Especially, I would mention Mr. Ng Be Cheer,
Mr. Sohaimi Abdullah and Mr. Mukhlis A. Rahman for their best efforts to guide me
on the technical part of my research. I owe my loving thanks to Mrs. Erna Yuliwati,
Ms. Nurul Hanan, Mr. Mohd. Abdul Razis Saidin, Mr. Azwar Azahari, Ms.
Norhaniza Yusof, Mr. Agung Mataram, Mrs. Nur Hidayati Othman, Dr. Lau Woei
Jye, Mrs. Tee Jia Chee, Mrs. Juhana Jaafar, Mrs. Hatijah Basri, Dr. Suhaila Sanip,
Ms. Goh Pei Sean, Ms. Nurul Saadah, Mrs. Farhana Aziz, Ms. Wan Norhayati, Ms.
Nur Atiqah, Ms. Safia Syazana, Dr. Mohd Noorul Anam, Dr. Amir Mansourizadeh,
Mr. Seyed Abdollatif and others that always be there with their undivided supports. I
also would like to express my sincere gratitude to all organizations that directly and
indirectly involved towards the success in producing this thesis. Mr. Mohd Fadzlee
Zainal Abidin and Mr. Mohamad Ibrahim Ahmad (AMREC SIRIM Berhad,
KULIM) thanks for your helping hand during my testing. I hope this thesis will
evoke an even greater response and be a valuable guide in the engineering field.
Above all, I thank Allah the Al-Mighty for bringing us together in the first place, and
my family for their patience and understanding.
The aims of this study were to prepare and characterize polyacrylonitrile
(PAN) fiber as a precursor for carbon fiber production. A dry-jet wet spinning
technique with a multi-hole spinneret (10 holes, = 0.350 mm) and a solvent-free
coagulation bath system were adopted in the preparation of PAN fibers precursor.
The spinning dope consisted of polymer polyacrylonitrile (PAN) with acrylamide
(AM) as an additive. Dimethylsulfoxide (DMSO) and dimethylformamide (DMF)
were employed as solvent in the dope formulation. The dopes were prepared at 18
wt.% polymer concentration and coagulation bath temperature was varied between
13 C to 20 C. The PAN fibers were characterized using field emission scanning
electron microscopy (FESEM), fourier transform infrared (FTIR), differential
scanning calorimetry (DSC), thermogravimetry (TGA), x-ray diffraction (XRD) and
tensile test. FESEM micrographs showed that at 18 wt.% of polymer concentration,
PAN fibers prepared from DMF and DMSO exhibited similar circular cross-sectional
structure with different fiber surfaces as coagulation bath temperature increased.
Dope prepared from DMF resulted on PAN fibers with rough fiber surface
meanwhile PAN fibers produced with DMSO showed smooth fiber surface. Both
PAN fibers prepared from DMF and DMSO showed the presence of typical
functional groups of precursor fibers particularly nitrile groups which is significant
for higher processing temperature. The lowest weight lost was observed
approximately 56 wt.% for PAN fibers prepared from DMSO. It showed a significant
improvement of the polymer stability which enhanced the carbon yield. The highest
glass transition temperature (Tg) recorded for PAN fibers fabricated from DMF was
92 C and both PAN fibers from DMF and DMSO solvents exhibited the highest
percentage of crystallinity which was 35 %. The mechanical properties of the
prepared fibers are strongly dependent on the type of solvent used during the
preparation. PAN fibers prepared from DMSO achieved the maximum of 279.20 kPa
on tensile strength while maximum 3.25 GPa Youngs modulus obtained by PAN
fibers prepared from DMF. This study concludes that different types of dope solvent
and variation of coagulation bath temperature played significant role to determine the
fiber structures and properties as well as fabricating PAN fibers via solvent-free
coagulation system. The results also elucidate that dry-jet wet spinning technique
with a multi-hole spinneret using solvent-free coagulation bath system with 18 wt.%
polymer concentration produced PAN fibers continuously without any breakage thus
enhanced the production of carbon fiber precursor.
Kajian ini adalah bertujuan untuk menghasilkan dan mencirikan gentian poliakrilonitril (PAN) sebagai prapenanda bagi pengeluaran gentian karbon. Teknik
pemutaran pancutan-kering basah yang terdiri daripada pemejam lubang berbilang (10
lubang, = 0.350 mm) dan sistem takungan pengentalan bebas pelarut telah digunakan
untuk penghasilan gentian PAN prapenanda. Larutan pemutaran terdiri daripada PAN
sebagai polimer, akrilamid (AM) sebagai bahan tambah. Dimetilformamid (DMF) dan
dimetilsulfoksida (DMSO) sebagai pelarut dalam formulasi larutan. Kepekatan polimer
disediakan pada 18 wt. % dan suhu takungan pengentalan diubahkan di antara 13 C hingga
20 C. Gentian PAN dicirikan dengan menggunakan mikroskopi imbasan electron
pemancaran medan (FESEM), spektroskopi inframerah transformasi fourier (FTIR),
pemeteran kalori pengimbasan kebezaan (DSC), analisis gravimetrik terma (TGA),
pembelauan X-ray (XRD) dan ujian tegangan. Mikrograf FESEM mendedahkan bahawa
pada kepekatan larutan polimer 18 wt.% gentian PAN yang disediakan dari DMF dan
DMSO mempamerkan struktur keratan rentas bulatan yang sama dengan permukaan gentian
yang berbeza semasa suhu takungan pengentalan ditingkatkan. Larutan yang dihasilkan
daripada pelarut DMF mempamerkan permukaan gentian yang kasar sementara larutan yang
dihasilkan daripada pelarut DMSO mempamerkan permukaan gentian yang licin. Kedua-dua
gentian PAN yang dihasilkan menggunakan pelarut DMF dan DMSO menunjukkan
kehadiran kumpulan berfungsi gentian PAN yang lazim terutama sekali kumpulan berfungsi
nitril amat penting untuk suhu pemprosesan yang tinggi. Kehilangan berat yang terendah
dimiliki oleh gentian PAN yang dihasilkan menggunakan pelarut DMSO iaitu dianggarkan
sebanyak 56 wt.%. Ia menunjukkan peningkatan yang ketara pada kestabilan polimer yang
telah meningkatkan penghasilan karbon. Suhu peralihan kaca (Tg) yang tertinggi adalah 92
C direkodkan oleh gentian PAN yang dihasilkan menggunakan larutan DMF. Kedua-dua
gentian PAN yang dihasilkan menggunakan larutan DMF dan DMSO mempamerkan peratus
kehabluran yang tertinggi sebanyak 35 %. Sifat mekanik gentian adalah sangat bergantung
kepada jenis pelarut yang digunakan semasa penyediaan larutan polimer. Dalam kajian ini,
maksimum kekuatan tegangan 279.20 kPa telah dicapai oleh gentian PAN yang dihasilkan
menggunakan pelarut DMSO sementara modulus Young yang maksimum ialah 3.25 GPa
telah dicapai oleh gentian PAN yang dihasilkan menggunakan pelarut DMF. Kajian ini
menunjukkan bahawa jenis pelarut dan suhu takungan pengentalan yang berbeza memainkan
peranan yang penting dalam menentukan struktur dan sifat gentian serta penghasilan gentian
PAN yang berkualiti melalui sistem takungan pengentalan bebas pelarut. Keputusan kajian
ini juga menunjukkan bahawa teknik pemutaran pancutan-kering basah bersama pemejam
lubang berbilang yang menggunakan sistem takungan pengentalan bebas pelarut dengan
kepekatan larutan polimer 18 wt.% telah berjaya menghasilkan gentian PAN secara
berterusan tanpa pematahan sepanjang pemprosesan pemutaran sambil meningkatkan
keluaran gentian prapenanda karbon.
TABLE OF CONTENTS
CHAPTER TITLE PAGE
TABLE OF CONTENTS vii
LIST OF TABLES xi
LIST OF FIGURES xiii
LIST OF ABBREVIATIONS xvi
LIST OF SYMBOLS xvii
LIST OF APPENDICES xviii
1.1 Research Background 1
1.2 Problem Statement 3
1.3 Research Objectives 5
1.4 Research Scopes 5
1.5 Significance of Study 6
2 LITERATURE REVIEW
2.1 History of Carbon Fiber 7
2.1.1 Carbon Fiber Today 8
2.1.2 Carbon Fiber Structure and Properties 10
2.1.3 Classification of Fibers 11
2.1.4 Applications of Carbon Fiber 13
2.2 Precursor for Carbon Fiber 16
2.2.1 Advantages and Disadvantages of Various
2.2.2 Polyacrylonitrile (PAN) 20
2.2.3 PAN as a Precursor Carbon Fiber 23
2.3 Spinning Techniques 24
2.3.1 Melt Spinning 24
2.3.2 Dry Spinning 25
2.3.3 Wet Spinning 25
2.3.4 Dry-jet Wet Spinning 26
2.4 Spinneret Design 28
2.4.1 Fiber Cross-sectional Shape 31
2.4.2 Skin-core Structure 32
2.4.3 Precursor Fiber Diameter 32
2.5 Spinning Conditions 33
2.5.1 Polymer Solution Formulation 33
2.5.2 Coagulation Process 38
2.5.3 Jet Stretch 40
2.6 Post Spinning Modifications 42
2.7 Conversion of PAN Fiber into PAN-based
2.7.1 Oxidative Stabilization 43
2.7.2 Carbonization 45
2.7.3 Graphitization 47
2.7.4 Carbon Fiber Surface Treatment 48
3 RESEARCH METHODOLOGY
3.1 Introduction 49
3.2 Experimental Flow 50
3.3 Material Selection 51
3.3.1 Polyacrylonitrile (PAN) 51
3.3.2 Dimethylformamide (DMF) and 52
3.3.3 Acrylamide (AM) 53
3.4 Polymer Solution Preparation 54
3.5 Fiber Spinning Apparatus and Procedures 55
3.6 Drying Process 56
3.7 Fiber Characterization Techniques and
3.7.1 Field Emission Scanning Electron
3.7.2 Fourier Transform Infra-Red Spectroscopy
3.7.3 X-ray Diffraction (XRD) 58
3.7.4 Differential Scanning Calorimetric (DSC) 58
3.7.5 Thermogravimetric Analysis (TGA) 59
3.7.6 Tensile Testing 60
4 RESULTS AND DISCUSSION
4.1 Introduction 61
4.2 The PAN Fiber Fabrication Process 63
4.3 Effects of Solvent Type 64
4.3.1 Spinning and Drying Process 64
4.3.2 Morphology and Structure of PAN Fibers 65
4.3.3 Void Formation 68
4.4 Effects of Coagulation Bath Temperature 69
4.4.1 Morphology and Structure of PAN Fibers 69
4.4.2 Void Formation 73
4.5 Effects of Residence Time 74
4.5.1 Spinning Process 74
4.5.2 Coagulation Bath Temperature 75
4.5.3 Void Formation 76
4.6 Fiber Diameter 77
4.6.1 Effects of Solvent Type 77
4.6.2 Effects of Coagulation Bath Temperature 78
4.7 FTIR Analysis of PAN Fibers 79
4.8 Thermal Analysis of PAN Fibers 82
4.8.1 Glass Transition Temperature 82
22.214.171.124 Effects of Solvent Type 82
126.96.36.199 Effects of Coagulation Bath
4.8.2 PAN Fiber Weight Loss 86
188.8.131.52 Effects of Solvent Type 86
184.108.40.206 Effects of Coagulation Bath
4.9 Effects of Solvent Types and Jet Stretch on the
Degree of Crystallization
4.10 Mechanical Properties of PAN Fibers 92
4.10.1 Effects of Void Formation 92
4.10.2 Effects of Coagulation Bath Temperature 93
5 CONCLUSION AND RECOMMENDATIONS
5.1 Conclusion 97
5.2 Recommendations for Future Work 99
LIST OF PUBLICATIONS 101
REFERENCES 102 110
APPENDICES 111 - 127
LIST OF TABLES
TABLE NO. TITLE PAGE
2.1 Groups of carbon fiber based on modulus 12
2.2 Classification of carbon fiber based on heat treatment
2.3 Carbon fiber applications and characteristics 15
2.4 Advantages and disadvantages of different type of
carbon fiber precursors
2.5 Possible comonomers for PAN precursors 22
2.6 Schematic of various spinning methods 27
2.7 Summary of various multi-hole spinneret
specifications from various researchers
2.8 Polymer concentrations used by various references 35
2.9 Various molecular weights of PAN based on various
2.10 Type of coagulants and its coagulation rate 39
3.1 Properties of polyacrylonitrile 51
3.2 Properties of dimethylformamide and
3.3 Properties of acrylamide 53
3.4 The dry-jet wet spinning specification 55
4.1 Residence times at different coagulation bath
4.2 Various fiber diameters based on solvent type and
various coagulation bath temperatures
4.3 Characteristics IR band of PAN fibers 82
4.4 Glass transition temperatures of PAN fibers prepared 84
from DMF and DMSO solvent at various coagulation
4.5 Total weight loss of PAN fibers prepared from DMF
4.6 XRD data of PAN fibers prepared with different
solvent types and various coagulation bath
4.7 Mechanical properties data of PAN fibers 93
LIST OF FIGURES
FIGURE NO. TITLE PAGE
1.1 The crystal structure of graphite 1
2.1 The prices and consumptions of carbon fiber based
on the applications
2.2 Relationship between precursor primary Youngs
modulus (Ep) and Youngs modulus of the resultant
carbon fibers (Ec)
2.3 Molecular structure of polyacrylonitrile 20
2.4 (a) Irregular helical structure of PAN (b)
Morphological model of PAN fiber showing ordered
and disordered regions
2.5 Schematics design of spinnerets (a) conventional (b)
and (c) present designed to avoid the formation of a
radial-type carbon fiber microstructure
2.6 Schematic of a skin core structure in a high speed
spun fiber showing a greater degree of crystallization
in the skin than in the core
2.7 Youngs modulus versus polymer solution
composition in the solvent-free coagulation bath
2.8 Flow chart represents the manufacturing of carbon
fibers from PAN fibers
2.9 Transformation structure of PAN into ladder PAN
when heat is applied
2.10 Transformation structure during (a) stabilization and
2.11 Schematic representation of carbon fiber structure (a) 47
Isotropic centre and oriented outer skin (b) Different
orientation in the centre and the outer layers (c) One
type of preferred orientation
2.12 Three dimensional model of carbon structure 48
3.1 The flow chart of fabrication and characterizations of
3.2 Polymer solution apparatus 54
3.3 Schematic diagram of advanced dry-jet wet spinning
4.1 Cross-sectional structures of PAN fiber (i) DMF and
(ii) DMSO solvent
4.2 Surfaces of PAN fiber with (a) DMF and (b) DMSO
4.3 Cross-sectional structures of PAN fiber with (i) DMF
and (ii) DMSO at different coagulation bath
temperature (a) 13 C (b) 16 C and (c) 20 C
4.4 Surfaces of PAN fiber with (i) DMF and (ii) DMSO
at different coagulation bath temperature (a) 13 C
(b) 16 C and (c) 20 C
4.5 IR spectrums of PAN fibers (DMF solvent) at various
coagulation bath temperature (A) 13 C (B) 16 C (C)
4.6 IR spectrums of PAN fibers (DMSO solvent) at
various coagulation bath temperatures (D) 13 C (E)
16 C (F) 20 C
4.7 DSC curves of PAN fibers with different types of
4.8 DSC curves of PAN fibers from DMF solvent at
various coagulation bath temperatures
4.9 DSC curves of PAN fibers from DMSO solvent at
various coagulation bath temperatures
4.10 TGA curves of PAN fibers with different types of
4.11 TGA curves of PAN fibers prepared from DMF
solvent at various coagulation temperatures
4.12 TGA curves of PAN fibers prepared from DMSO
solvent at various coagulation bath temperatures
4.13 The change in (a) tensile strength and (b) Youngs
modulus with coagulation bath temperature of PAN
fibers prepared with DMF and DMSO solvent
LIST OF ABBREVIATIONS
PAN - Polyacrylonitrile
UHM - Ultra-high-modulus
HM - High-modulus
IM - Intermediate-modulus
HT - High-tensile
SHT - Super high-tensile
HTT - Heat treatment temperature
DMF - Dimethylformamide
DMSO - Dimethylsulphoxide
FRP - Fiber reinforced plastics
AM - Acrylamide
DMAc - Dimethylacetamide
NaSCN - Natrium thiocyanate
ZnCl2 - Zinc Chloride
CuCl2 - Cuprum Chloride
CH4 - Methane
H2 - Hydrogen
HCN - Hydrogen cyanide
H2O - Water
O2 - Oxygen
CO - Carbon monoxide
CO2 - Carbon dioxide
NH3 - Ammonia
FTIR - Fourier transform infra-red spectroscopy
XRD - X-ray diffraction
TGA - Thermogravimetric analysis
DSC - Differential scanning calorimetric
LIST OF SYMBOLS
% - Percent
C - Degree Celcius
GPa - Giga Pascal
kPa - Kilo Pascal
ca - Circa
Ec - Elastic modulus of carbon fibers
Ep - Elastic modulus of precursor fibers
wt. % - Weight percent
- Jet stretch
> - More than
< - Less than
GHz - Giga Hertz
g/cm3 - Gram per centimeter cubic
Cp - Centipoise
N - Newton
m - Micrometer
nm - Nanometer
mm - Milimeter
mg - Miligrams
mm/min - Milimeter per minute
C/min - Degree per minute
Ac - Area under the crystalline diffraction peaks
Aa - Area under the amorphous zone
Tg - Glass transition temperature
LIST OF APPENDICES
APPENDIX TITLE PAGE
A Spinning Process Specification 111
B IR Spectra of PAN Fibers 113
C Thermal Properties of PAN Fibers 117
D X-ray Diffraction Curves 124
1.1 Research Background
Carbon fibers are very thin black fibers. It can be much thinner than human
hair. Each carbon filament thread is a bundle of many thousand carbon filaments. A
single such filament is a thin fiber with a diameter of 5 to 8 micrometers and consists
almost exclusively of carbon. Carbon fibers consist of 99.9 % of chemically pure
carbon (Fitzer, 1985). They can be short or continuous. Their structure can be
crystalline, amorphous or partly crystalline (Chung, 1994). The crystalline form has
the crystal structure of graphite as shown in Figure 1.1.
Figure 1.1 The crystal structure of graphite: a direction is parallel to the basal
planes and b direction is perpendicular to the basal planes (Morgan, 2005)
Historically, there are three types of carbon fiber precursors: 1) cellulose
(rayon), 2) mesophase pitch and 3) polyacrylonitrile (PAN) (Buckley and Edie,
1993). Carbon fibers from cellulose (rayon) precursor are no longer produced
because of the high cost of conversion to carbon. Furthermore, the reaction is more
complicated than just simple dehydration and the carbon yield is only of the order of
25-30 %. Pitch precursor, however has a higher yield of 85 % with a high resultant
modulus but due to their more graphitic nature, they will have poorer compression.
At present, all commercial carbon fibers are produced from PAN precursor.
Carbon fiber properties are significantly dependant on the precursor
properties. In order to convert precursor to carbon fiber, three basic requirements of
precursor are needed, i.e. (1) it should be easily converted to carbon fiber, (2) it
offers a high carbon yield and (3) it allows to be processed economically. PAN has
become the attraction as a precursor because of its continuous carbon backbone and
the nitrile groups are ideally placed for cyclization reaction to occur which forms
ladder structure to enable them throughout higher processing temperatures (Rahaman
et al., 2007; Sedghi et al., 2008).
Generally, precursor fibers can be fabricated by various methods such as wet
spinning, dry spinning, melt spinning and dry-jet wet spinning. Subsequently,
precursor fibers will undergo heat treatment processes. Heat treatment process is
significant as it is a conversion stage of precursor fibers into carbon fibers. There are
normally three successive stages involving oxidation or stabilization in air,
carbonization in an inert environment and graphitization. Precursor fibers are first
stretched and simultaneously oxidized in the temperature range of 200-300 C
(Minus and Kumar, 2005; Kannadaguli and Rong, 2004). At this stage, ladder
structure will form to allow them to be processed at higher temperature. After
oxidation, the fibers are then carbonized in the range of 1000 C to 1700 C in an
inert atmosphere (Minus and Kumar, 2005). During this heating process the non-
carbon elements are removed as volatiles and yield a turbostatic structure. Finally,
the fibers are treated at temperature 1500 C to 3000 C depending on the fiber type
all through graphitization to further improve the basal planes orientation and fiber
1.2 Problem Statement
Carbon fibers have been popularly used worldwide as replacement for steel
and metal as an alternative material for reinforcement usage. Intensive researches
have been continuously carried out to produce an excellent quality of carbon fibers.
Dong X-G et al. (2007) and Jain et al. (1987) reported that the properties of carbon
fibers mainly depend on the quality of the precursor fibers. There are few precursors
that can be used to produce carbon fiber such as polyacrylonitrile, pitch and rayon.
Polyacrylonitrile has been found to be the most suitable precursor to obtain
carbon fiber with excellent performance (Wang Y-X et al., 2007a). About 90 % of
the carbon fibers produced are made from PAN fibers (Rahman et al., 2007;
Rahaman et al., 2007; Gupta and Harrison, 1996). PAN-based carbon fiber generally
has a higher tensile strength than a fiber based on any other precursors due to its high
melting point, thermally stable, low weight loss during heat treatments and a high
degree of molecular orientation (Mukhlis, 2006).
In spite of all the advantages mentioned on the PAN fiber, there are
drawbacks in achieving good mechanical properties of PAN-based carbon fiber.
There are the spinning difficulties involving factors such as polymer solution
concentration, dope viscosity, coagulation bath temperature and residence time.
Finding the optimum polymer solution concentration is a critical factor, in order to
successfully spin the fiber. Ji et al. (2007) reported that higher polymer content
accompanies the increase of the viscosity whereas Bahrami et al. (2003) reported that
with an increase in the concentration of the polymer in the dope the spinnability can
be improved, the tenacity increased and the porosity reduced in the cross section of
the fiber. Increasing the polymer concentration improves the homogeneity of the
fiber structure by reducing the generation of large voids, increasing the density and
slightly improving the tenacity (Knudsen, 1963).
Dope viscosity also plays an important role in the spinnability of PAN fiber.
A very low viscosity may lead to dope fracture whereas a high viscosity may slow
down the spinning speed and coagulation rate (Bajaj et al., 2002). Both, coagulation
bath temperature and residence time as well have a huge effect on the coagulation
process. Coagulation bath temperature is responsible for controlling the mass-
transfer and the counter-diffusion of the solvent and non-solvent thus influences
microscopic and morphological structures as well as mechanical properties of PAN
fibers (Rahman et al., 2007; Bahrami et al., 2003; Bajaj et al., 2002). Rahman et al.
(2007) reported that a short residence time prevented further inward diffusion of non-
solvent towards the center of PAN fibers and the higher the residence time, the more
non-solvent diffuses towards the PAN fibers.
The drawback of conventional technique is the high amount of solvent
content in the coagulation bath to fabricate PAN fibers for carbon fibers production
which could probably cause cancer for a long period of exposure as well as damage
the system (Ismail et al., 2008). In addition, it would increase the electrical
consumption. According to Bajaj et al. (2002), dry-jet wet spinning technique
improves the PAN fibers mechanical properties. Work by Mukhlis (2006) showed
that dry-jet wet spinning process via solvent-free coagulation bath with a single-hole
spinneret has been successfully carried out and produced PAN fibers with
competitive mechanical properties. However, the use of a single-hole spinneret is
impractical as it has to take long time to produce PAN fibers precursor in bundle.
The big volume of precursor fibers is needed especially during tensile and
application testing. Tagawa and Miyata (1997) reported that for composites
reinforced, carbon fibers were used in continuous form. Moreover, there is still no
study reported on the usage of multi-hole spinneret via solvent-free coagulation bath
to produce PAN fibers. Most of previous studies demonstrated that the use of a
multi-hole spinneret with high concentration of solvent content in the coagulation
bath to produce PAN fibers (Bahrami et al., 2003; Bajaj et al. 2002).
The present study further investigated the use of a multi-hole spinneret and
improved the understanding of spinning conditions in solvent-free coagulation bath
and to enhance the PAN-based carbon fiber performance and production. Therefore,
this study attempts to prepare and characterize PAN fiber precursor with certain
polymer concentration for carbon fiber production using a multi-hole spinneret along
with the suitability of dry-jet wet spinning conditions.
1.3 Research Objectives
Based on the above problem statements, the objectives of this research are:
(i) To study the effects of the different types of solvent used in the dope
solution formulation on the structural of PAN fibers with a multi-hole
(ii) To study the effects of coagulation bath temperature, residence time
and solvent-free coagulation bath on the structure of PAN fibers.
(iii) To investigate the characteristics of PAN fibers based on the
morphology and mechanical properties.
1.4 Research Scopes
In order to achieve the above mentioned objectives, the scopes of this
research have been identified:
(i) Preparation of several spinning solutions using DMF and DMSO
solvent, respectively and study on the 18 wt.% polymer concentration
in fabricating PAN fibers using dry-jet wet spinning technique with a
multi-hole spinneret (10 holes) in the solvent-free coagulation bath.
(ii) Investigating the effects of solvent type used during dope solution
formulation on the PAN fibers structure.
(iii) Investigating the effects of coagulation bath temperature by varying
the coagulation bath temperature at 13 C, 16 C and 20 C on the
morphological structure of PAN fiber.
(iv) Characterizing the PAN fibers based on the Field Emission Scanning
Electron (FESEM), Fourier Transform Infrared (FTIR), X-ray
Diffraction (XRD), Differential Scanning Electron (DSC),
Thermogravimetric (TGA) and Tensile Test machine for the PAN
1.5 Significance of Study
The significance of the present study are:
(i) PAN fibers precursor fabricated using dry-jet wet spinning with multi-
hole spinneret in a solvent-free coagulation system is potential in fiber
technology due to the reduction of time consumption as well as
enhance the fiber production.
(ii) The solvent-free coagulation bath system could be considered for
fabricating PAN fibers precursor as it allows the precursor fibers to be
processed economically due to the usage of 100 % water in the
coagulation bath as well as minimizing the environmental issue.
(iii) Using solvent-free coagulation bath with multi-hole spinneret, the
PAN fibers resulted in an acceptable Youngs modulus of 3.25 GPa
compared to Rahman et al. (2007) study of 2.93 GPa.
Bahrami, S.H., Bajaj, P., and Sen, K. (2003). Effect of Coagulation Conditions on
Properties of Poly(acrylonitrile-carboxylic acid) Fibers. Journal of Applied
Polymer Science, Vol.89, 1825-1837.
Bai, Y-J., Wang, C-G., Lun, N., Wang, Y-X., Yu, M-J., and Zhu, B. (2006). HRTEM
Microstructures of PAN Precursor Fibers. Carbon, Vol. 44, 1773-1778.
Bajaj, P., Sreekumar, T.V., and Sen, K. (2002). Structure Development during Dry-
Jet-Wet Spinning of Acrylonitrile/Vinyl Acids and Acrylonitrile/Methyl
Acrylate Copolymers. Journal of Applied Polymer Science, Vol.86, 773-787.
Balasubramanian, M., Jain, M.K., Bhattacharya, S.K., and Abhiraman, A.S. (1987).
Conversion of Acrylonitrile-based Precursors to Carbon Fibers Part 3:
Thermooxidative Stabilization and Continuous, Low Temperature
Carbonization. Journal of Materials Science, Vol. 22, 3864-3872.
Baojun, Q., Ding, P., and Zhenqiou, W. (1986). The Mechanism and Characteristics
of Dry-Jet Wet-Spinning of Acrylic Fibers. Journal of Advances in Polymer
Technology, Vol.6, No.4, 509-529.
Buckley, J.D., and Edie, D.D. (1993). Carbon-Carbon Materials and Composites.
New Jersey: Noyes Publications.
Chawla, K.K. (1998). Fibrous Materials. England: The Press Syndicate of University
Chen, J.C., and Harrison, I.R. (2002). Modification of Polyacrylonitrile (PAN)
Carbon Fiber Precursor via Post-spinning Plasticization and Stretching in
Dimethylformamide (DMF). Carbon, Vol. 40, 25-45.
Chung, D.D.L. (1994). Carbon Fiber Composites. Boston: Butterworth-Heinemann
Dong, R., Keuser, M., Zeng, X., Zhao, J., Zhang, Y., Wu, C., and Pan, D. (2008).
Viscometric Measurement of the Thermodynamics of PAN
Terpolymer/DMSO/Water System and Effect of Fiber-Forming Conditions
on the Morphology of PAN Precursor. Journal of Polymer Science, Vol. 46,
Dong, X-G., Wang, C-G., Bai, Y-J., and Cao, W-W. (2007). Effect of DMSO/H2O
Coagulation Bath on the Structure and Property of Polyacrylonitrile Fibers
during Wet-Spinning. Journal of Applied Polymer Science, Vol.105, 1221-
Dong, X-G., Wang, C-G., Chen, J., and Cao, W-W. (2008). Crystallinity
Development in Polyacrylonitrile Nascent Fibers during Coagulation. Journal.
Polymer Research, Vol. 15, 125-130.
Donnet, J.B., and Bansal, R.C. (1984). Carbon Fibers. New York: Marcel Dekker
Donnet, J.B., Rebouillat, S., Wang, T.K., and C.M.Peng, J. (Eds.) (1998). Carbon
ed.). New York: Marcel Dekker Inc.
Doppert, H.L., and Harmsen, G.J. (1973). The Influence of the Stretch Ratio on the
Rate of Diffusion in a Wet-Spinning Process. Journal of Applied Polymer
Science, Vol.17, 893-903.
E-Composite, Growth Opportunities in Carbon Fiber Composites Market 2006
2011, E-Composites, Inc. 2006.
Edie, D.D. (1998). The Effect of Processing on the Structure and Properties of
Carbon Fibers. Carbon, Vol.36, No.4, 345-362.
Farsani, R.E., Shokuhfar, A., and Sedghi, A. (2007). Conversion of Modified
Commercial Polyacrylonitrile Fibers to Carbon Fibers. International Journal
of Mechanical Systems Science and Engineering 1, 4 182-185.
Fitzer, E. (Ed.) (1985). Carbon Fibres and Their Composites. Berlin: Springer-
Gabbott, P. (2008). Principles and Applications of Thermal Analysis. Blackwell
Galasso, F.S. (1989). Advanced Fibers and Composites. Gordon and Breach Science
Gupta, A., and Harrison, I.R. (1996). New Aspects in the Oxidative Stabilization of
PAN-based Carbon Fibers. Carbon, Vol.34, No. 11, 1427-1445.
Gupta, A.K., and Maiti, A.K. (1982). Effect of Heat Treatment on the Structure and
Mechanical Properties of Polyacrylonitrile Fibers. Journal of Applied
Polymer Science, Vol.27, 2409-2416.
Gupta, B., Revagade, N., Anjum, N., Atthoff, B., and Hilborn, J. (2006). Preparation
of Poly(lactic acid) Fiber by Dry-Jet-Wet-Spinning. I. Influence of Draw
Ratio on Fiber Properties. Journal of Applied Polymer Science, Vol.100,
Han, C.D. and Park, J.Y. (1973). A Study of Shaped Fiber Formation. Journal of
Applied Polymer Science, Vol. 17, 187-200.
He, D-X., Wang, C-G., Bai, Y-J., Lun, N., Zhu, B., and Wang, Y-X. (2007).
Microstructural Evolution during Thermal Stabilization of PAN Fibers.
Journal Material Science, Vol. 42, 7402-7407.
Hou, C., Liang, Y., and Wang, C-G. (2005). Determination of the Diffusion
Coefficient of H2O in Polyacrylonitrile Fiber Formation. Journal of Polymer
Research, Vol. 12, 49-52.
Hou, C., Qu, R., Wang, C., and Ying, L. (2006). Diffusion Coefficient of DMF in
Acrylic Fiber Formation. Journal of Applied Polymer Science, Vol. 101,
Howard, W.H. (1961). Glass Temperatures of Polyacrylonitrile and Acrylonitrile
Vinyl Acetate Copolymers. Journal of Applied Polymer Science, Vol. V, 303-
Http://www.carbonfibrechina.com. Large tow for carbon fiber manufacturer.
Retrieved on 21st February 2008.
Http://www.merck.de/. Material safety data sheet (MSDS) for dimethylformamide
and dimethylsulfoxide. Retrieved on 13th
fibre-market/. Retrieved on 15th
Http://www.sigmaaldrich.com. Material safety data sheet (MSDS) for
polyacrylonitrile and acrylamide. Retrieved on 8th
Huang, X., (2009). Fabrication and Properties of Carbon Fibers. Materials, Vol. 2,
Ismail A.F., Rahman M.A., Mustafa A., and Matsuura T. (2008). The Effect of
Processing Conditions on a Polyacrylonitrile Fiber Produced using a Solvent-
free Coagulation Process. Journal of Materials Science and Engineering A,
Vol. 485, 251-257.
Jain, M.K., and Abhiraman, A.S. (1987). Conversion of Acrylonitrile-based
Precursor Fibres to Carbon Fibres Part 1: A Review of the Physical and
Morphological Aspects. Journal of Materials Science, Vol. 22, 278-300.
Ji, B-H., Wang, C-G., and Wang, Y-X. (2007). Effect of Jet Stretch on
Polyacrylonitrile As-Spun Fiber Formation. Journal of Applied Polymer
Science, Vol. 103, 3348-3352.
Ji, B-H., Wang, J-H., Wang, C-G., and Wang, Y-X. (2008). Study on the Formation
Process of Polyacrylonitrile As-Spun Fiber. Journal of Applied Polymer
Science, Vol.108, 328-333.
Ji, M., Wang, C., Bai, Y., Yu, M., and Wang, Y. (2007). Structural Evolution of
Polyacrylonitrile Precursor Fibers during Preoxidation and Carbonization.
Polymer Bulletin, Vol. 59, 527-536.
Kannadaguli, M., and Rong, H. (2004). Carbon Fibers (Updated: April 2004)
Kim, C., Cho, Y.J., Yun, W.Y., Ngoc, B.T.N., Yang, K.S., Chang, D.R., Lee, J.W.,
Kojima, M., Kim, Y.A., and Endo, M. (2007). Fabrications and Structural
Characterization of Ultra-fine Carbon Fibres by Electrospinning of Polymer
Blends. Solid State Communications, Vol. 142, 20-23.
Knudsen, J.P. (1963). The Influence of Coagulation Variables on the Structure and
Physical Properties of an Acrylic Fiber. Textile Research Journal, Vol. 33,
Ko T-H, (1994). The Influence of Pyrolisis on Physical Properties and
Microstructure of Modified PAN fibers during Carbonization. Journal of
Applied Polymer Science, Vol.43, 589-600.
Kobashi, T. and Takao, S. (1987). Method for the Production of High Strength
Polyacrylonitrile Fiber. (U.S. Patent 4,659,529).
Kobayashi, Y., Okajima, S., and Kosuda, H. (1967). Change of Orientation by
Thermal Contraction of Polyacrylonitrile Fiber, Journal of Applied Polymer
Science, Vol. 11, 2525-2531.
Krigbaum, W.R., and Tokita, N. (1960). Melting Point Depression Study of
Polyacrylonitrile. Journal of Polymer Science, Vol. XLIII, 467-488.
Kruchinin, N.P., Spirova, T.A., Medvedev, A.T., Serkov, A.T., Radishevskii, M.B.,
Volodin, V.I., Prokhorov, V.A., Krutova, I.N., Egorova, and Grekhova E.V.
(1991). Morphological and Structural Features of Polyacrylonitrile Fibers
Spun by the Dry-wet Method. Khimicheskie Volokna, No. 3, pp.19-22.
Langley, M. (1973). Carbon Fibers In Engineering. United Kingdom, McGraw Hill
Lee, K.J., and Chen, Z.Y. (2003). Microstructure Study of PAN-pitch-based Carbon-
carbon Composite. Materials Chemistry and Physics, Vol. 82, 428-434.
Liu, F., Wang, H., Xue, L., Fan, L., and Zhu, Z. (2008). Effect of Microstructure on
the Mechanical Properties of PAN-based Carbon Fibers during High-
temperature Graphitization. Journal of Materials Science, Vol. 43, 4316-
Liu, J-J., Ge, H., and Wang, C-G. (2006). Modification of Polyacrylonitrile
Precursors for Carbon Fiber via Copolymerization of Acrylonitrile with
Ammonium Itaconate. Journal of Applied Polymer Science, Vol.102, 2175-
Loidl, D., Paris, O., Rennhofre, H., Muller, M. and Peterlik, H. (2007). Skin-core
structure and Bimodal Weibull Distribution of the Strength of Carbon Fibers.
Carbon 45, 2801-2805.
Mikolajczyk, T., Bogun, M., and Kowalczyk, A. (2005). Effect of Fibre-spinning
Conditions on the Properties of Nanosilica-containing Precursor PAN Fibres.
July/September 2005, Vol.13, No.3. 30-34.
Min, B. G., Sreekumar, T.V., Uchida, T., Kumar, S. (2005). Oxidative Stabilization
of PAN/SWNT Composite Fiber. Carbon, Vol. 43, 599-604.
Minus, M.L., and Kumar, S. February (2005). The Processing, Properties, and
Structure of Carbon Fibers. Overview High-Performance Fibers, 52-58.
Mittal, J., Mathur, R.B., and Bahl, O.P. (1997). Post Spinning Modification of PAN
Fibres-A Review. Carbon, Vol.35, No.12, 1713-1722.
Mittal, J., Mathur, R.B., Bahl, O.P., and Inagaki, M. (1998). Post Spinning Treatment
of PAN Fibers using Succinic Acid to Produce High Performance Carbon
Fibers. Carbon, Vol. 36, 893-897.
Moreton, R., and Watt, W. (1974). The Spinning of Polyacrylonitrile Fibres in Clean
Room Conditions for the Production of Carbon Fibres. Carbon, Vol. 12, 543-
Morgan, P. (2005). Carbon Fibers and Their Composites. Boca Raton: Taylor and
Muhammad Syukri Bin Abd. Rahaman (2006). Development and Characterization of
Carbon Fiber from Polyacrylonitrile Precursor. M.Sc. Thesis. Universiti
Teknologi Malaysia, Skudai.
Mukhlis Bin A. Rahman (2006). Effects of Fabrication Conditions in the Solvent-
Free Coagulation Process on the Structural and Mechanical Properties of
Polyacrylonitrile/Acrylamide Fibers. M.Sc. Thesis. Universiti Teknologi
Ouyang, Q., Cheng, L., Wang, H., and Li, K. (2008). Mechanism and Kinetics of the
Stabilization Reactions of Itaconic Acid-modified Polyacrylonitrile. Polymer
Degradation and Stability, Vol. 93, 1415-1421.
Padhye, M.R., and Karandikar, A.V. (1987). Effect of Thermal and Solvent
Treatment on the Viscoelastic Behavior of PAN Fiber in the Glass-Rubber
Transition Region. Journal of Applied Polymer Science, Vol. 33, 1675-1682.
Pakshver, E.A., Semenova, N.A., and Neverov, A.P. (1977). Glass Transition
Temperature of As-spun Polyacrylonitrile Fibre. Plenum Publishing
Corporation. No. 2, 40-41.
Paul, D.R. (1968a). A Study of Spinnability in the Wet-spinning of Acrylic Fibers.
Journal of Applied Polymer Science, Vol. 12, 2273-2298.
Paul, D.R. (1968b). Diffusion During the Coagulation Step of Wet-Spinning. Journal
of Applied Polymer Science, Vol.12, 383-402.
Peng, G-Q., Wen, Y-F., Yang, Y-G., Liu, L., and Wang, W. (2009) Effect of Dope
Extrustion Rate on the Formation and Characterization of Polyacrylonitrile
Nascent Fibers during Wet- Spinning. Polymer Bulletin. 62, 657-666.
Pfeiffer, R.E., and Peacher S.E. (1980). Process for Melt-spinning Acrylonitrile
Polymer Fiber. (U.S. Patent 4,220,617).
Preta, I.F.C., Sakata, S.K., Garcia, G., Zimmermann, J.P., Galembeck, F., and
Giovedi, C. (2007). Thermal Behavior of Polyacrylonitrile Polymers
Synthesized under Different Conditions and Comonomer Compositions.
Journal of Thermal Analysis and Calorimetry, Vol. 87, 657-659.
Rahaman, M.S.A., Ismail, A.F., and Mustafa, A. (2007). A Review of Heat
Treatment on Polyacrylonitrile Fiber. Journal of Polymer Degradation and
Stability, Vol. 92, 1421-1432.
Rahman, M.A., Ismail, A.F., and Mustafa, A. (2007). The Effect of Residence Time
on the Physical Characteristics of PAN-based Fibers Produced using a
Solvent-free Coagulation Process. Journal of Material Science and
Engineering A, Vol. 448, 275-280.
Reichardt, M., Pieper, C.,Nogaj, A., Sandhu, S.S., and Grtner, E. (1983). Process
for the Production of High-strength Filaments from Dry-spun
Polyacrylonitrile. (U.S. Patent 4,421,708).
Rosenbaum, S. (1965). Polyacrylonitrile Fiber Behavior. I. Mechanisms of Tensile
Response. Journal of Applied Polymer Science, Vol. 9, 2071-2084.
Saufi, M.S. and Ismail, A.F. (2002). Development and Characterization of
Polyacrylonitrile (PAN) Based Carbon Hollow Fiber Membrane.
Songklanakarin Journal Science Technology, 843-854.
Sedghi, A., Farsani, R. E., and Shofukor, A. (2008). The Effect of Commercial
Polyacrylonitrile Fibers Characterizations on the Produced Carbon Fibers
Properties. Journal of Materials Processing Technology, Vol. 198, 60-67.
Seymour, R.B., and Porter, R.S. (1993). Manmade Fibers: Their Origin and
Development, Elsevier Science Publisher Ltd.
Shimada, T.O., and Imai, K. and Miyahara, N. (1990). Process for Preparing a
Carbon Fiber of High Strength. (U.S. Patent 4,925,604).
Shimamura, M., Minakuchi, H., Sakai, H., Kuwabara, T., Yuki, K., Abe, T., and all
of Iyo-gun. (1971). Process for the Preparation of Acrylic Fibers with Odd-
shaped Sections. (U.S. Patent 3,621,087).
Simitzis, J., and Soulis, S. (2008). Correlation of Chemical Shrinkage of
Polyacrylonitrile Fibres with Kinetics of Cyclization. Polymer International,
Vol. 57, 99-105.
Smith, C. (2001). Environmental Physics. Published by Routledge Taylor & Francis
Soon Wai Loon (2006). Effects of Coagulation Temperature and Polymer
Concentration on the Morphology and Mechanical Properties of
Polyacrylonitrile Precursor Fiber Fabricated through Solvent-Free
Coagulation Process. B.Eng. Thesis. Universiti Teknologi Malaysia, Skudai.
Stoyanov, A.I. (1982). Influence of the Content of Polymer with Different Molecular
Weights in Spinning Solutions on Properties of Acrylic Fibers. Journal of
Applied Polymer Science, Vol. 27, 235-238.
Tagawa, T., and Miyata, T. (1997). Size Effect on Tensile Strength of Carbon Fibers.
Material Science and Engineering A238, 336-342.
Tan, L., Chen, H., Pan, D., and Pan, N. (2008). Investigating the Spinnability in the
Dry-Jet Wet Spinning of PAN Precursor Fiber. Journal of Applied Polymer
Science, Vol. 110, 1997-2000.
Tsai, J-S and Wu, C.J. (1993). Effect of Cross-section Evenness for Polyacrylonitrile
Precursor on the Properties of Carbon Fibre. Journal of Material Science
Letters 12, 411-413.
Tsai, J-S. (1994). Orientation Change for Polyacrylonitrile Precursor during
Oxidation. Journal of Materials Science Letters 13, 1162-1163.
Tsai, J-S., and Lin, C-H. (1991a). Effect of Comonomer Composition on the
Properties of Polyacrylonitrile Precursor and Resulting Carbon Fiber. Journal
of Applied Polymer Science. Vol. 43, 679-685.
Tsai, J-S., and Lin, C-H. (1991b). The Effect of Molecular Weight on the Cross
Section and Properties of Polyacrylonitrile Precursor and Resulting Carbon
Fiber. Journal of Applied Polymer Science, Vol. 42, 3045-3050.
Walczak, Z.K. (1977). Formation of Synthetic Fibers, Gordon and Breach Science
Wang, C-G., Dong, X-G and Wang, Q-F. (2009). Effect of Coagulation on the
Structure and Property of PAN Nascent Fibers during Dry Jet Wet-spinning.
Journal Polymer Research, Vol.16, 719-724.
Wang, Y-X., Wang, C-G., and Yu, M-J. (2007b). Effects of Different Coagulation
Conditions on Polyacrylonitrile Fibers Wet Spun in a System of
Dimethylsulphoxide and Water. Journal of Applied Polymer Science, Vol.
Wang, Y-X., Wang, C-G., Wu, J-W., and Jing, M. (2007a). High Temperature DSC
Study of Polyacrylonitrile Precursors during Their Conversion to Carbon
Fibers. Journal of Applied Polymer Science, Vol.106, 1787-1792.
Wangxi, Z., Jie, L., and Gang, W. (2003). Evolution of Structure and Properties of
PAN Precursors during Their Conversion to Carbon Fibers. Carbon, Vol. 41,
Warner, S.B., Uhlmann, D.R. and Peebles, L.H. (1979). Oxidative Stabilization of
Acrylic Fibres. Journal of Materials Science, Vol. 14, 1893-1900.
Wu, G.P., Lu, C.X., Zhang, R., Wu, X.P., Ren, F.Z., Li, K.X., He, F., and Ling, L.C.
(2004). Effect of Moisture on Stabilization of Polyacrylonitrile Fibers.
Journal of Materials Science, Vol. 39, 2959-2960.
Ying, L., Hou, C., and Qun, W. (2007). Rheological Behavior of
Acrylonitrile/Ammonium Acrylate Copolymer Solutions. Journal of Applied
Polymer Science, Vol.103, 2320-2324.
Yu, M., Wang, C. Bai, Y., Wang, Y., and Xu, Y. (2006a). Influence of Precursor
Properties on the Thermal Stabilization of Polyacrylonitrile Fibers. Polymer
Bulletin 57, 757-763.
Yu, M., Wang, C., Bai, Y., Wang, Y., and Zhu, B. (2006b). Evolution of Tension
during the Thermal Stabilization of Polyacrylonitrile Fibers under Different
Parameters. Journal of Applied Polymer Science, Vol. 102, 5500-5506.
Zeng, X.., Hu, J., Zhao, J., Zhang, Y., and Pan, D. (2007). Investigating the Jet
Stretch in the Wet Spinning of PAN Fiber. Journal of Applied Polymer
Science, Vol.106, 2267-2273.